#------------------------------------------------------------------------------
#$Date: 2019-11-22 22:24:58 +0200 (Fri, 22 Nov 2019) $
#$Revision: 231424 $
#$URL: file:///home/coder/svn-repositories/cod/cif/4/00/32/4003201.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4003201
loop_
_publ_author_name
'McKellar, Scott C.'
'Sotelo, Jorge'
'Greenaway, Alex'
'Mowat, John P. S.'
'Kvam, Odin'
'Morrison, Carole A.'
'Wright, Paul A.'
'Moggach, Stephen A.'
_publ_section_title
;
 Pore Shape Modification of a Microporous Metal--Organic Framework Using
 High Pressure: Accessing a New Phase with Oversized Guest Molecules
;
_journal_issue                   2
_journal_name_full               'Chemistry of Materials'
_journal_page_first              466
_journal_paper_doi               10.1021/acs.chemmater.5b02891
_journal_volume                  28
_journal_year                    2016
_chemical_formula_moiety         'C28.50 H12 O12 Sc2'
_chemical_formula_sum            'C28.5 H12 O12 Sc2'
_chemical_formula_weight         636.31
_space_group_IT_number           70
_space_group_name_Hall           '-F 2uv 2vw'
_space_group_name_H-M_alt        'F d d d :2'
_symmetry_cell_setting           orthorhombic
_symmetry_Int_Tables_number      70
_symmetry_space_group_name_Hall  '-F 2uv 2vw'
_symmetry_space_group_name_H-M   'F d d d :2'
_atom_sites_solution_hydrogens   difmap
_atom_sites_solution_primary     other
_audit_creation_date             15-06-08
_audit_creation_method           CRYSTALS_ver_14.40
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.779(3)
_cell_length_b                   20.742(3)
_cell_length_c                   34.287(7)
_cell_measurement_reflns_used    1723
_cell_measurement_temperature    293
_cell_measurement_theta_max      23
_cell_measurement_theta_min      3
_cell_volume                     6243(3)
_computing_cell_refinement       'Apex2 (Bruker AXS, 2006)'
_computing_data_collection       'Apex2 (Bruker AXS, 2006)'
_computing_data_reduction        'Apex2 (Bruker AXS, 2006)'
_computing_molecular_graphics    'CAMERON (Watkin et al., 1996)'
_computing_publication_material  'CRYSTALS (Betteridge et al., 2003)'
_computing_structure_refinement  'CRYSTALS (Betteridge et al., 2003)'
_computing_structure_solution    'Superflip (Palatinus & Chapuis, 2007)'
_diffrn_ambient_pressure         200000
_diffrn_ambient_temperature      293
_diffrn_measured_fraction_theta_full 0.719
_diffrn_measured_fraction_theta_max 0.671
_diffrn_measurement_device       Area
_diffrn_measurement_device_type  'Bruker Kappa Apex2'
_diffrn_measurement_method       ω
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.090
_diffrn_reflns_limit_h_max       6
_diffrn_reflns_limit_h_min       -6
_diffrn_reflns_limit_k_max       22
_diffrn_reflns_limit_k_min       -22
_diffrn_reflns_limit_l_max       35
_diffrn_reflns_limit_l_min       -35
_diffrn_reflns_number            4145
_diffrn_reflns_theta_full        17.426
_diffrn_reflns_theta_max         23.234
_diffrn_reflns_theta_min         3.086
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    0.493
_exptl_absorpt_correction_T_max  0.95
_exptl_absorpt_correction_T_min  0.77
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'SADABS (Siemens, 1996)'
_exptl_crystal_colour            colourless
_exptl_crystal_density_diffrn    1.354
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       block
_exptl_crystal_F_000             2568
_exptl_crystal_size_max          0.200
_exptl_crystal_size_mid          0.100
_exptl_crystal_size_min          0.100
_refine_diff_density_max         0.59
_refine_diff_density_min         -0.60
_refine_ls_extinction_coef       8.524
_refine_ls_extinction_method     'Larson (1970), Equation 22'
_refine_ls_goodness_of_fit_ref   0.8839
_refine_ls_hydrogen_treatment    noref
_refine_ls_matrix_type           full
_refine_ls_number_parameters     113
_refine_ls_number_reflns         753
_refine_ls_number_restraints     149
_refine_ls_R_factor_all          0.0973
_refine_ls_R_factor_gt           0.0579
_refine_ls_shift/su_max          0.0012940
_refine_ls_shift/su_mean         0.0000277
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
;
 Method, part 1, Chebychev polynomial, (Watkin, 1994, Prince, 1982) 
 [weight] = 1.0/[A₀*T₀(x)+A₁*T₁(x) ... +Aₙ₋₁]*Tₙ₋₁(x)] 
 where Ai are the Chebychev coefficients listed below and x= Fcalc/Fmax 
 Method = Robust Weighting (Prince, 1982) 
 W = [weight] * [1-(deltaF/6*sigmaF)²]² 
 Ai are: 
 9.42 12.3 6.05 1.84 
;
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_all         0.1602
_refine_ls_wR_factor_gt          0.1284
_refine_ls_wR_factor_ref         0.1602
_reflns_limit_h_max              6
_reflns_limit_h_min              0
_reflns_limit_k_max              22
_reflns_limit_k_min              0
_reflns_limit_l_max              35
_reflns_limit_l_min              0
_reflns_number_gt                530
_reflns_number_total             760
_reflns_threshold_expression     I>2.0σ(I)
_oxford_diffrn_Wilson_B_factor   0.00
_oxford_diffrn_Wilson_scale      0.00
_oxford_refine_ls_r_factor_ref   0.0973
_oxford_refine_ls_scale          0.04993(3)
_oxford_reflns_number_all        753
_oxford_reflns_threshold_expression_ref I>-3.0\s(I)
_oxford_structure_analysis_title 'ST2135s in Fddd'
_cod_data_source_file            cm5b02891_si_003.cif
_cod_data_source_block           SC2BDC3_np_I
_cod_depositor_comments
;
The following automatic conversions were performed:

data item '_atom_sites_solution_primary' value 'Other' was changed to
'other' in accordance with the
/home/saulius/struct/COD-crude-data/automatic-downloads/DataCite-retrospective/ACS/depositions/lib/dictionaries/cif_core.dic
dictionary named 'cif_core.dic' version 2.4.2 last updated on
2011-04-26.

Automatic conversion script
Id: cif_fix_values 6909 2019-04-08 15:41:33Z antanas 
;
_cod_original_cell_volume        6244(2)
_cod_original_sg_symbol_H-M      'F d d d'
_cod_original_formula_sum        'C28.50 H12 O12 Sc2'
_cod_database_code               4003201
_iucr_refine_instruction_details_constraints
;
#
# Punched on 08/06/15 at 13:42:45
#
#LIST     12                                                                    
BLOCK X'S 
CONT SCALE 
CONT SC   (1 ,U'S)  UNTIL C(8) 
CONT C (10, U[ISO]) UNTIL C(14) 
END                                                                             
;
_iucr_refine_instruction_details_restraints
;
#
# Punched on 08/06/15 at 13:42:45
#
#LIST     16                                                                    
NO 
DIST 1.39, 0.01 = C(6) TO C(7), C(7) TO C(8) 
CONT              C(8) TO C(6,4,2,0,0,-1) 
PLANAR 0.010000  C(6) C(7) C(8) C(6,4,2,0,0,-1) 
REM   HREST   START (DO NOT REMOVE THIS LINE) 
REM   HREST   END (DO NOT REMOVE THIS LINE) 
REM   DELU   START (DO NOT REMOVE THIS LINE) 
VIBR .0, 0.00200 = O(1) TO C(1) 
VIBR .0, 0.00200 = O(2) TO C(1) 
VIBR .0, 0.00200 = O(3) TO C(5) 
VIBR .0, 0.00200 = C(1) TO C(2) 
VIBR .0, 0.00500 = O(2) TO O(1) 
VIBR .0, 0.00500 = C(2) TO O(1) 
VIBR .0, 0.00500 = C(2) TO O(2) 
VIBR .0, 0.00200 = C(2) TO C(4,-1,4,0,0,1) 
VIBR .0, 0.00200 = C(2) TO C(3) 
VIBR .0, 0.00500 = C(4,-1,4,0,0,1) TO C(1) 
VIBR .0, 0.00500 = C(3) TO C(1) 
VIBR .0, 0.00500 = C(3) TO C(4,-1,4,0,0,1) 
VIBR .0, 0.00200 = C(3) TO C(4) 
VIBR .0, 0.00500 = C(4) TO C(2) 
VIBR .0, 0.00500 = C(2,-1,4,0,0,1) TO C(3) 
VIBR .0, 0.00200 = C(5) TO C(6) 
VIBR .0, 0.00500 = O(3,-3,1,0,0,1) TO O(3) 
VIBR .0, 0.00500 = C(6) TO O(3) 
VIBR .0, 0.00500 = C(6) TO O(3,-3,1,0,0,1) 
VIBR .0, 0.00200 = C(6) TO C(8,-2,1,0,1,1) 
VIBR .0, 0.00200 = C(6) TO C(8,4,2,0,0,-1) 
VIBR .0, 0.00200 = C(6) TO C(7,-3,1,0,0,1) 
VIBR .0, 0.00200 = C(6) TO C(7) 
VIBR .0, 0.00500 = C(8,-2,1,0,1,1) TO C(5) 
VIBR .0, 0.00500 = C(8,4,2,0,0,-1) TO C(5) 
VIBR .0, 0.00500 = C(8,4,2,0,0,-1) TO C(8,-2,1,0,1,1) 
VIBR .0, 0.00500 = C(7,-3,1,0,0,1) TO C(5) 
VIBR .0, 0.00500 = C(7,-3,1,0,0,1) TO C(8,-2,1,0,1,1) 
VIBR .0, 0.00500 = C(7,-3,1,0,0,1) TO C(8,4,2,0,0,-1) 
VIBR .0, 0.00500 = C(7) TO C(5) 
VIBR .0, 0.00500 = C(7) TO C(8,-2,1,0,1,1) 
VIBR .0, 0.00500 = C(7) TO C(8,4,2,0,0,-1) 
VIBR .0, 0.00500 = C(7) TO C(7,-3,1,0,0,1) 
VIBR .0, 0.00200 = C(7) TO C(8,-2,1,0,1,1) 
VIBR .0, 0.00200 = C(7) TO C(8) 
VIBR .0, 0.00500 = C(8,-2,1,0,1,1) TO C(6) 
VIBR .0, 0.00500 = C(8) TO C(6) 
VIBR .0, 0.00500 = C(8) TO C(8,-2,1,0,1,1) 
VIBR .0, 0.00200 = C(8) TO C(8,-2,1,0,1,1) 
VIBR .0, 0.00500 = C(7) TO C(6,-2,1,0,1,1) 
VIBR .0, 0.00500 = C(8,-2,1,0,1,1) TO C(6,-2,1,0,1,1) 
VIBR .0, 0.00500 = C(8,-2,1,0,1,1) TO C(7) 
VIBR .0, 0.00500 = C(7,-2,1,0,1,1) TO C(6,-2,1,0,1,1) 
VIBR .0, 0.00500 = C(7,-2,1,0,1,1) TO C(7) 
VIBR .0, 0.00500 = C(7,-2,1,0,1,1) TO C(8,-2,1,0,1,1) 
REM   DELU   END (DO NOT REMOVE THIS LINE) 
REM   THERMSIM   START (DO NOT REMOVE THIS LINE) 
U(IJ) .0, 0.08000 = O(1) TO C(1) 
U(IJ) .0, 0.08000 = O(2) TO C(1) 
U(IJ) .0, 0.04000 = O(3) TO C(5) 
U(IJ) .0, 0.04000 = C(1) TO C(2) 
U(IJ) .0, 0.04000 = C(2) TO C(4,-1,4,0,0,1) 
U(IJ) .0, 0.04000 = C(2) TO C(3) 
U(IJ) .0, 0.04000 = C(3) TO C(4) 
U(IJ) .0, 0.04000 = C(5) TO C(6) 
U(IJ) .0, 0.04000 = C(6) TO C(8,-2,1,0,1,1) 
U(IJ) .0, 0.04000 = C(6) TO C(8,4,2,0,0,-1) 
U(IJ) .0, 0.04000 = C(6) TO C(7,-3,1,0,0,1) 
U(IJ) .0, 0.04000 = C(6) TO C(7) 
U(IJ) .0, 0.04000 = C(7) TO C(8,-2,1,0,1,1) 
U(IJ) .0, 0.04000 = C(7) TO C(8) 
U(IJ) .0, 0.04000 = C(8) TO C(8,-2,1,0,1,1) 
REM   THERMSIM   END (DO NOT REMOVE THIS LINE) 
DISTANCE 2.40000 , 0.010000 = C(13) TO C(7,-2,2) 
U(IJ) .0, 0.04000 = C(10) TO C(11) 
U(IJ) .0, 0.04000 = C(11) TO C(12) 
U(IJ) .0, 0.04000 = C(12) TO C(13) 
U(IJ) .0, 0.04000 = C(13) TO C(14) 
U(IJ) .0, 0.04000 = C(14) TO C(15) 
U(IJ) .0, 0.04000 = C(15) TO C(15,-1,4) 
VIBRATION 0.0, 0.020000 = C(10) TO C(11) 
VIBRATION 0.0, 0.020000 = C(11) TO C(12) 
VIBRATION 0.0, 0.020000 = C(12) TO C(13) 
VIBRATION 0.0, 0.020000 = C(13) TO C(14) 
VIBRATION 0.0, 0.020000 = C(14) TO C(15) 
VIBRATION 0.0, 0.020000 = C(15) TO C(15,-1,4) 
DISTANCE 1.540000 , 0.010000 = C(10) TO C(11) 
DISTANCE 1.540000 , 0.010000 = C(11) TO C(12) 
DISTANCE 1.540000 , 0.010000 = C(12) TO C(13) 
DISTANCE 1.540000 , 0.010000 = C(13) TO C(14) 
DISTANCE 1.540000 , 0.010000 = C(14) TO C(15) 
DISTANCE 1.540000 , 0.010000 = C(15) TO C(15,-1,4) 
ANGLE 113.000000 , 1.000000 = C(11,-2) TO C(10) TO C(11) 
ANGLE 113.000000 , 1.000000 = C(10) TO C(11) TO C(12) 
ANGLE 113.000000 , 1.000000 = C(11) TO C(12) TO C(13) 
ANGLE 113.000000 , 1.000000 = C(12) TO C(13) TO C(14) 
ANGLE 113.000000 , 1.000000 = C(13) TO C(14) TO C(15) 
ANGLE 113.000000 , 1.000000 = C(14) TO C(15) TO C(15,-1,4) 
END                                                                             
;
loop_
_symmetry_equiv_pos_as_xyz
x,y,z
-x,-y,-z
x,y+1/2,z+1/2
-x,-y+1/2,-z+1/2
x+1/2,y,z+1/2
-x+1/2,-y,-z+1/2
x+1/2,y+1/2,z
-x+1/2,-y+1/2,-z
-x,y+1/4,z+1/4
x,-y+1/4,-z+1/4
-x,y+3/4,z+3/4
x,-y+3/4,-z+3/4
-x+1/2,y+1/4,z+3/4
x+1/2,-y+1/4,-z+3/4
-x+1/2,y+3/4,z+1/4
x+1/2,-y+3/4,-z+1/4
x+1/4,-y,z+1/4
-x+1/4,y,-z+1/4
x+1/4,-y+1/2,z+3/4
-x+1/4,y+1/2,-z+3/4
x+3/4,-y,z+3/4
-x+3/4,y,-z+3/4
x+3/4,-y+1/2,z+1/4
-x+3/4,y+1/2,-z+1/4
-x+1/4,-y+3/4,z+1/2
x+1/4,y+3/4,-z+1/2
-x+1/4,-y+5/4,z+1
x+1/4,y+5/4,-z+1
-x+3/4,-y+3/4,z+1
x+3/4,y+3/4,-z+1
-x+3/4,-y+5/4,z+1/2
x+3/4,y+5/4,-z+1/2
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_occupancy
_atom_site_adp_type
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
Sc1 Sc 0.3750 0.3750 0.63577(5) 0.0142 1.0000 Uani S T
O1 O 0.2459(8) 0.3344(3) 0.59262(16) 0.0447 1.0000 Uani . U
O2 O 0.0091(8) 0.3332(2) 0.57028(14) 0.0345 1.0000 Uani . U
O3 O 0.2430(8) 0.4582(2) 0.63522(18) 0.0416 1.0000 Uani . U
C1 C 0.1484(13) 0.3203(3) 0.5677(2) 0.0265 1.0000 Uani . U
C2 C 0.2021(11) 0.2837(4) 0.5324(2) 0.0345 1.0000 Uani . U
C3 C 0.0963(13) 0.2642(5) 0.5045(2) 0.0526 1.0000 Uani . U
C4 C 0.1478(14) 0.2306(5) 0.4722(2) 0.0520 1.0000 Uani . U
C5 C 0.1250 0.4862(4) 0.6250 0.0285 1.0000 Uani S TU
C6 C 0.1250 0.5581(4) 0.6250 0.0351 1.0000 Uani DS TU
C7 C 0.2555(14) 0.5895(7) 0.6374(3) 0.0559 0.5000 Uani D U
C8 C 0.2514(15) 0.6565(8) 0.6370(3) 0.0532 0.5000 Uani D U
C10 C 0.6250 0.1660(5) 0.1250 0.39(5) 0.2500 Uiso DS U
C11 C 0.6250 0.1250 0.0876(3) 0.39(5) 0.5000 Uiso DS U
C12 C 0.526(6) 0.1538(18) 0.0549(8) 0.40(5) 0.2500 Uiso D U
C13 C 0.366(3) 0.123(5) 0.0527(10) 0.41(5) 0.2500 Uiso D U
C14 C 0.277(14) 0.144(8) 0.016(4) 0.42(5) 0.2500 Uiso D U
H3 H -0.0090 0.2736 0.5077 0.0631 1.0000 Uiso . .
H4 H 0.0770 0.2173 0.4529 0.0624 1.0000 Uiso . .
H7 H 0.3431 0.5665 0.6458 0.0671 0.5000 Uiso . .
H8 H 0.3393 0.6794 0.6454 0.0638 0.5000 Uiso . .
loop_
_atom_type_symbol
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_Cromer_Mann_a1
_atom_type_scat_Cromer_Mann_b1
_atom_type_scat_Cromer_Mann_a2
_atom_type_scat_Cromer_Mann_b2
_atom_type_scat_Cromer_Mann_a3
_atom_type_scat_Cromer_Mann_b3
_atom_type_scat_Cromer_Mann_a4
_atom_type_scat_Cromer_Mann_b4
_atom_type_scat_Cromer_Mann_c
_atom_type_scat_source
C 0.0033 0.0016 2.3100 20.8439 1.0200 10.2075 1.5886 0.5687 0.8650 51.6512
0.2156 'International Tables Vol C 4.2.6.8 and 6.1.1.4'
H 0.0000 0.0000 0.4930 10.5109 0.3229 26.1257 0.1402 3.1424 0.0408 57.7998
0.0030 'International Tables Vol C 4.2.6.8 and 6.1.1.4'
O 0.0106 0.0060 3.0485 13.2771 2.2868 5.7011 1.5463 0.3239 0.8670 32.9089
0.2508 'International Tables Vol C 4.2.6.8 and 6.1.1.4'
Sc 0.2519 0.3716 9.1890 9.0213 7.3679 0.5729 1.6409 136.1080 1.4680 51.3531
1.3329 'International Tables Vol C 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_site_symmetry_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle_site_symmetry_3
_geom_angle
_geom_angle_publ_flag
O2 18_556 Sc1 O2 16_556 88.3(3) yes
O2 18_556 Sc1 O3 29_554 88.6(2) yes
O2 16_556 Sc1 O3 29_554 92.1(2) yes
O2 18_556 Sc1 O1 29_554 179.5(3) yes
O2 16_556 Sc1 O1 29_554 92.2(3) yes
O3 29_554 Sc1 O1 29_554 91.5(2) yes
O2 18_556 Sc1 O1 . 92.2(3) yes
O2 16_556 Sc1 O1 . 179.5(3) yes
O3 29_554 Sc1 O1 . 87.8(3) yes
O1 29_554 Sc1 O1 . 87.3(4) yes
O2 18_556 Sc1 O3 . 92.1(2) yes
O2 16_556 Sc1 O3 . 88.6(2) yes
O3 29_554 Sc1 O3 . 179.0(3) yes
O1 29_554 Sc1 O3 . 87.8(3) yes
O1 . Sc1 O3 . 91.5(2) yes
Sc1 . O1 C1 . 167.1(6) yes
Sc1 16_456 O2 C1 . 133.2(5) yes
Sc1 . O3 C5 . 149.1(5) yes
O2 . C1 O1 . 125.0(7) yes
O2 . C1 C2 . 117.9(7) yes
O1 . C1 C2 . 117.1(10) yes
C1 . C2 C4 8_556 120.4(7) yes
C1 . C2 C3 . 119.3(9) yes
C4 8_556 C2 C3 . 120.3(7) yes
C2 . C3 C4 . 118.5(10) yes
C2 . C3 H3 . 120.8 no
C4 . C3 H3 . 120.8 no
C3 . C4 C2 8_556 121.3(8) yes
C3 . C4 H4 . 119.4 no
C2 8_556 C4 H4 . 119.4 no
O3 . C5 O3 18_556 124.2(9) yes
O3 . C5 C6 . 117.9(4) yes
O3 18_556 C5 C6 . 117.9(4) yes
C5 . C6 C8 27_554 121.8(8) yes
C5 . C6 C8 10_566 121.8(8) yes
C8 27_554 C6 C8 10_566 116.5(17) yes
C5 . C6 C7 18_556 118.0(8) yes
C8 27_554 C6 C7 18_556 35.3(5) yes
C8 10_566 C6 C7 18_556 108.7(8) yes
C5 . C6 C7 . 118.0(8) yes
C8 27_554 C6 C7 . 108.7(8) yes
C8 10_566 C6 C7 . 35.3(5) yes
C7 18_556 C6 C7 . 123.9(17) yes
C6 . C7 C7 10_566 104.6(7) yes
C6 . C7 C8 10_566 72.8(8) yes
C7 10_566 C7 C8 10_566 54.4(17) yes
C6 . C7 C8 . 116.4(15) yes
C7 10_566 C7 C8 . 29.5(7) yes
C8 10_566 C7 C8 . 84(2) yes
C6 . C7 H7 . 121.8 no
C7 10_566 C7 H7 . 125.9 no
C8 10_566 C7 H7 . 112.5 no
C8 . C7 H7 . 121.8 no
C8 10_566 C8 C6 10_566 106.7(7) yes
C8 10_566 C8 C7 . 32.8(8) yes
C6 10_566 C8 C7 . 123.4(15) yes
C8 10_566 C8 C7 10_566 63.4(17) yes
C6 10_566 C8 C7 10_566 71.9(8) yes
C7 . C8 C7 10_566 96(2) yes
C8 10_566 C8 H8 . 125.6 no
C6 10_566 C8 H8 . 118.3 no
C7 . C8 H8 . 118.3 no
C7 10_566 C8 H8 . 102.5 no
C11 18_655 C10 C10 27_644 56.5(5) yes
C11 18_655 C10 C11 . 112.9(9) yes
C10 27_644 C10 C11 . 56.5(5) yes
C12 27_644 C11 C10 10_555 113.1(9) yes
C12 27_644 C11 C10 . 145(2) yes
C10 10_555 C11 C10 . 67.1(9) yes
C12 27_644 C11 C12 . 86(3) yes
C10 10_555 C11 C12 . 145(2) yes
C10 . C11 C12 . 113.1(9) yes
C11 . C12 C13 . 113.0(9) yes
C12 . C13 C14 . 112.9(9) yes
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_site_symmetry_2
_geom_bond_distance
_geom_bond_publ_flag
Sc1 O2 18_556 2.100(5) yes
Sc1 O2 16_556 2.100(5) yes
Sc1 O3 29_554 2.079(5) yes
Sc1 O1 29_554 2.044(6) yes
Sc1 O1 . 2.044(6) yes
Sc1 O3 . 2.079(5) yes
O1 C1 . 1.244(11) yes
O2 C1 . 1.255(11) yes
O3 C5 . 1.238(7) yes
C1 C2 . 1.506(10) yes
C2 C4 8_556 1.359(14) yes
C2 C3 . 1.392(13) yes
C3 C4 . 1.385(10) yes
C3 H3 . 0.950 no
C4 H4 . 0.950 no
C5 C6 . 1.493(12) yes
C6 C8 27_554 1.392(8) yes
C6 C8 10_566 1.392(8) yes
C6 C7 18_556 1.385(8) yes
C6 C7 . 1.385(8) yes
C7 C7 10_566 1.70(3) yes
C7 C8 10_566 0.842(12) yes
C7 C8 . 1.390(8) yes
C7 H7 . 0.950 no
C8 C8 10_566 1.55(3) yes
C8 H8 . 0.950 no
C10 C11 18_655 1.538(9) yes
C10 C10 27_644 1.70(2) yes
C10 C11 . 1.538(9) yes
C11 C12 27_644 1.538(9) yes
C11 C12 . 1.538(9) yes
C12 C13 . 1.539(9) yes
C13 C14 . 1.540(9) yes
loop_
_oxford_refln_omitted_index_h
_oxford_refln_omitted_index_k
_oxford_refln_omitted_index_l
_oxford_refln_omitted_flag
1 3 25 x
2 4 30 x
